Monodisperse Hollow Tricolor Pigment Particles for Electronic Paper
© to the authors 2009
Received: 31 August 2009
Accepted: 2 October 2009
Published: 25 October 2009
A general approach has been designed to blue, green, and red pigments by metal ions doping hollow TiO 2. The reaction involves initial formation of PS at TiO2 core–shell nanoparticles via a mixed-solvent method, and then mixing with metal ions solution containing PEG, followed calcining in the atmosphere. The as-prepared hollow pigments exhibit uniform size, bright color, and tunable density, which are fit for electronic paper display.
KeywordsE-paper Pigment Hollow Bistable
In the past few years, electronic paper (E-paper), which is a display technology based on the electrophoresis of charged particles, has recently been enthusiastically investigated with regard to not only their potential application in planar display, but also the fundamental understanding of nanoscopic phenomena [1–6]. There are many benefits over other display technologies, such as low-power consumption, good flexibility, low weight and high reflexivity and contrast [7–10].
Ever since E-paper was first prepared, the performance of electronic paper has been rapidly improved, as a result of technological development and the accumulation of fundamental knowledge. Despite tremendous advances, one of the common challenges for all the electronic paper techniques is to achieve full-color E-paper . For colorization, color filters decrease the contrast and brightness. A pixel composed of tricolor unites, in which red, blue, and green particles are suspended in a fluid medium, respectively, is a promising design. Thereby, it is necessary to prepare tricolor pigment particles. For E-paper display, the pigments should be bistable . By applying the voltage, the pigments move, while stopping the voltage, it will hold still. The pigments will keep at the position until applying a voltage. In the case, the matching of the pigments with the dielectric medium is a key factor. There have been a few early attempts at achieving the objectives. It involves polymer coating on pigments or polymer–pigment hybrid ; however, these pigments are limited as the polymer decreases the color gamut. In this article, a solution for the problem will be given while we prepare hollow pigments.
Here, a facile general method, which is based on the tuning of the bandgap of semiconductor by metal ions doping is developed to prepare monodisperse hollow tricolor pigment particles. Titania and Cr 2+ metal ions are selected as host materials and dopants, respectively. The obtained green hollow pigment samples (Cr 3+ doped TiO2), are well characterized by using X-ray diffraction (XRD), scanning electron microscope (SEM), transmission electron microscopy (TEM), and UV–vis diffuse reflection. They show brilliant colors in visible region. And the density of hollow pigment particles is about 1.32 g/cm 3, which is very low and can match well with most of dispersants. By the method, we can also prepare other metal ions doped TiO2 hollow nanocomposites, such as Co/Al doped TiO2 hollow particles (blue), Fe doped TiO2 hollow particles (red). The monodisperse hollow tricolor pigment particles are potential building blocks to fabricate full-color electrophoretic display.
Tetra-n-butyl titanate (TBT) and acetonitrile were purchased from Sigma and used without further purification. Potassium persulfate (KPS), FeCl 36H2O, CrCl 3 6H2O, Al (NO3)39H2O, Polyethylene glycol (PEG 10000), styrene, ethanol, and ammonia were all supplied by the Beijing Chemical Reagent Company. Styrene was purified by distillation under reduced pressure. Ethanol was dehydrated by molecule sieves.
The monodisperse metal ions doped TiO2 hollow particles were prepared by using the Pechini sol–gel process. Anionic polystyrene (PS) spheres used as core materials were prepared by emulsifier-free, emulsion polymerization using KPS as the anionic initiator. TiO2 coating on the as-prepared PS core was processed in the mixed solvent of ethanol and acetonitrile by hydrolyzing TBT in the presence of ammonia, as described in our previous report . 1.2 mmol CrCl 36H2O was first dissolved in a water–ethanol (1/7 v/v) solution containing citric acid which was two times as much as the metal ions in amount of substance. And then a certain amount of the PEG (10000) was added. The solution was stirred for 2 h and then the above PS/TiO2 hybrid spheres (0.04 g) were added. After stirring for another 4 h, the particles were separated by centrifugation. The samples were dried at 60 °C for 2 h and then annealed at 500 °C for 4 h with a heating rate of 5 °C/min. Finally the preheated samples were annealed at 600 °C for 2 h with a heating rate of 2 °C/min.
TEM (JEOL-200CX) and SEM (Hitachi 4300) were used to observe the morphology of the particles. XRD measurement was employed a Japan Regaku D/max γA X-ray diffractometer equipped with graphite monochromatized Cu Kα radiation (λ = 1.54 ) irradiated with a scanning rate of 0.02 deg/s. Ultraviolet and visible absorption (UV–vis) and diffuse reflectance spectra were recorded at room temperature with the JASCO 570 spectrophotometer equipped with an integrated sphere.
Results and Discussion
E-paper is a straightforward fusion of chemistry, physics, and electronics. The pigments are very important to the E-paper properties [15–17]. In the interest of a full-color electronic paper, the tricolor particles are required. For green hollow nanospheres, PS at TiO2 core–shell nanoparticles are synthesized by a mixed-solvent method, and then mixed with Cr 3+ ions in the solution containing PEG, followed calcined in the atmosphere. The monodisperse Cr 3+-doped TiO2 hollow particles are prepared by using the Pechini sol–gel process by varying the condition, such as ratio of Cr 3+ ions to PS at TiO2 and the concentration of PEG. During the reaction, the chelate complexes of metal ions react with PEG to form polyesters with suitable viscosity, which coat on the surfaces of the PS/TiO2 particles.
where Q r, η, and E represent the charge, particle radius, viscosity of the suspension, and the potential difference applied to the suspension, respectively. The suspension viscosity can be considered constant in suspension. Under this condition, the electrophoretic velocity is mainly a function of the electric field and the particle size. As the particles in the suspension used for E-paper usually have a distribution of particle sizes, particles with different r value have different electrophoretic mobility, thereby resulting in the segregation effects observed during the display process. From the equation, we know that the particles with the same size shuttle between the up and down side of a pixel simultaneously. Thus, the uniform Cr 3+-doped TiO2 hollow particles will improve display properties.
The monodisperse Cr3+-doped TiO2 hollow particles are prepared by using the Pechini sol–gel process, in which PS at TiO2 core–shell nanoparticles are synthesized by a mixed-solvent method, and then mixed with Cr3+ in the solution containing PEG, followed calcined in the atmosphere. Fe3+-doped TiO2(red) and Co2+/Al3+-doped TiO2(blue) hollow nanocomposites are also prepared by this method. The hollow pigments are good candidates for full-color E-paper display.
The financial support for this research was provided by the Hi-Tech Research and Development Program of China (863) (2009AA03Z322), and the National Natural Science Foundation of China (60736001).
- Comiskey B, Albert JD, Hidekazu Y: Nature. 1998, 394: 253. COI number [1:CAS:528:DyaK1cXkvVGqtrw%3D]; Bibcode number [1998Natur.394..253C] 10.1038/28349View ArticleGoogle Scholar
- Jo GR, Hoshino K, Kitamura T: Chem. Mater.. 2002, 14: 664. COI number [1:CAS:528:DC%2BD38XmslChtA%3D%3D] 10.1021/cm010664nView ArticleGoogle Scholar
- Hayes RA, Feenstra BJ: Nature. 2003, 425: 383. COI number [1:CAS:528:DC%2BD3sXnsV2ktL4%3D]; Bibcode number [2003Natur.425..383H] 10.1038/nature01988View ArticleGoogle Scholar
- Wang JP, Zhao XP, Guo HL: Optical Mater.. 2008, 30: 1268. COI number [1:CAS:528:DC%2BD1cXjsF2hsrY%3D]; Bibcode number [2008OptMa..30.1268W] 10.1016/j.optmat.2007.05.057View ArticleGoogle Scholar
- Bot T, De Smet H, Beunis F, Neyts K: Displays. 2006, 27: 50. 10.1016/j.displa.2005.10.001View ArticleGoogle Scholar
- Arsenault AC, Puzzo DP, Manners I, Ozin GA: Nat. Photon.. 2007, 1: 468. COI number [1:CAS:528:DC%2BD2sXpsVentrw%3D]; Bibcode number [2007NaPho...1..468A] 10.1038/nphoton.2007.140View ArticleGoogle Scholar
- Lee JY, Sung JH, Jang IB: Synth. Met.. 2005, 153: 221. COI number [1:CAS:528:DC%2BD2MXpvVGktbk%3D] 10.1016/j.synthmet.2005.07.278View ArticleGoogle Scholar
- Wang YT, Zhao XP, Wang DW: J. Microencapsu1e. 2006, 23: 762. COI number [1:CAS:528:DC%2BD2sXjsFektg%3D%3D] 10.1080/02652040600788197View ArticleGoogle Scholar
- Kim CA, Joung MJ, Ahn SD: Synth. Met.. 2005, 151: 181. COI number [1:CAS:528:DC%2BD2MXms1Oksb4%3D] 10.1016/j.synthmet.2005.03.008View ArticleGoogle Scholar
- Bot T, De Smet H: Displays. 2003, 24: 223. 10.1016/j.displa.2004.01.009View ArticleGoogle Scholar
- Puzzo DP, Arsenault AC, Manners I, Ozin GA: Angew. Chem. Int. Ed.. 2008, 47: 1. 10.1002/anie.200790254View ArticleGoogle Scholar
- Bot T, De Smet H: Displays. 2003, 24: 103. 10.1016/j.displa.2003.09.001View ArticleGoogle Scholar
- Yu DG, An JH, Bae JY, Ahn SD, Kang SY, Suh KS: Macromolecules. 2005, 38: 7485. COI number [1:CAS:528:DC%2BD2MXmsVymt78%3D]; Bibcode number [2005Mamol..38.7485Y] 10.1021/ma035613lView ArticleGoogle Scholar
- Wang P, Chen D, Tang FQ: Langmuir. 2006, 22: 4832. COI number [1:CAS:528:DC%2BD28Xjt1Kmurs%3D] 10.1021/la060112pView ArticleGoogle Scholar
- Kang HS, Cha HJ, Kim JC: Mol. Cryst. Liq. Cryst.. 2007, 472: 247. COI number [1:CAS:528:DC%2BD2sXhtFeiu7jN]View ArticleGoogle Scholar
- Jang IB, Sung JH, Choi HJ: Synth. Met.. 2005, 152: 9. COI number [1:CAS:528:DC%2BD2MXpvVGksbk%3D] 10.1016/j.synthmet.2005.07.087View ArticleGoogle Scholar
- Peng B, Tang FQ, Chen D, Ren XL, Meng XW, Ren J: J. Colloid Interf. Sci.. 2009, 329: 62. COI number [1:CAS:528:DC%2BD1cXhtlCkt7jK] 10.1016/j.jcis.2008.09.069View ArticleGoogle Scholar
- Meng XW, Kwon TY, Yang YZ, Ong JL, Kim KH: J. Biomed. Mater. Res. B. 2006, 78B: 373. COI number [1:CAS:528:DC%2BD28XnvFWls74%3D] 10.1002/jbm.b.30497View ArticleGoogle Scholar